Survey

* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project

Transcript

PHYSICAL REVIEW B 77, 155410 共2008兲 CO oxidation on Pd(100) at technologically relevant pressure conditions: First-principles kinetic Monte Carlo study Jutta Rogal,* Karsten Reuter, and Matthias Scheffler Fritz-Haber-Institut der Max-Planck-Gesellschaft, Faradayweg 4-6, D-14195 Berlin, Germany 共Received 30 January 2008; revised manuscript received 14 March 2008; published 8 April 2008兲 The possible significance of oxide formation for the catalytic activity of transition metals in heterogeneous oxidation catalysis has evoked a lively discussion over the recent years. On the more noble transition metals 共such as Pd, Pt, or Ag兲, the low stability of the common bulk oxides primarily suggests subnanometer thin oxide films, so-called surface oxides, as potential candidates that may be stabilized under gas phase conditions representative of technological oxidation catalysis. We address this issue for the Pd共100兲 model catalyst surface with first-principles kinetic Monte Carlo simulations that assess the stability of the well-characterized 共冑5 ⫻ 冑5兲R27° surface oxide during steady-state CO oxidation. Our results show that at ambient pressure conditions, the surface oxide is stabilized at the surface up to CO : O2 partial pressure ratios just around the catalytically most relevant stoichiometric feeds 共pCO : pO2 = 2 : 1兲. The precise value sensitively depends on temperature, so that both local pressure and temperature fluctuations may induce a continuous formation and decomposition of oxidic phases during steady-state operation under ambient stoichiometric conditions. DOI: 10.1103/PhysRevB.77.155410 PACS number共s兲: 68.43.Bc, 82.65.⫹r, 68.43.De, 68.35.Md I. INTRODUCTION The large difference in catalytic activity of “ruthenium” catalysts toward CO oxidation under ultrahigh vacuum and ambient pressure conditions1 has recently been controversially discussed in terms of a possible oxide formation at the surface in technologically relevant environments.2,3 The well known much lower thermodynamic stability of the bulk oxides of Pd or Pt 共Ref. 4兲 suggests at first glance that this discussion has no direct relevance for these more noble metals that are equally, if not more often, used in oxidation catalysis. By using a constrained first-principles thermodynamics approach5 we showed in a preceding study,6 however, that the situation is not that clear-cut when considering the possibility of subnanometer thin oxide films, so-called surface oxides. By mapping out a wide range of 共T , pO2 , pCO兲 conditions, we specifically found for the Pd共100兲 surface that the stability range of the well-characterized 共冑5 ⫻ 冑5兲R27° 共冑5 in brevity兲 surface oxide structure7–11 does, indeed, extend up to pressure and temperature conditions relevant for technological CO oxidation catalysis 共T = 300– 600 K, pO2 = pCO ⬃ 1 atm兲. This insight motivates to center a detailed kinetic modeling of the surface structure and the composition during steady-state CO oxidation at technologically relevant pressure conditions on the 冑5 surface oxide. More precisely, the question of a possible oxide formation at the surface can be narrowed down to addressing the stability, formation, and decomposition of the 冑5 surface oxide structure in the reactive environment. Theoretically, one is then still faced with the challenge to evaluate the kinetics of the surface elementary processes over time scales of the order of seconds or longer, while accurately accounting for the evolving atomistic structure of the surface. In this study, we meet the timescale challenge with a first-principles statistical mechanics approach, combining density-functional theory 共DFT兲 for an accurate description of the kinetic parameters with kinetic Monte Carlo 共kMC兲 simulations for the evaluation of the 1098-0121/2008/77共15兲/155410共12兲 nonequilibrium statistical mechanics problem. At present, such an approach is preferentially carried out on the basis of a lattice model for the surface in order to keep the number of required DFT-based parameters tractable. Due to the different periodicity and Pd density of the 冑5 overlayer6,12,13 and the Pd共100兲 substrate, a combined lattice model embracing both structures will be highly involved and will require numerous kinetic parameters for a manifold of conceivable atomistic pathways for the complex structural transition between oxidized and pristine Pd surfaces. Before embarking on such an explicit modeling of the formation and decomposition of the surface oxide structure in the simulations, it is thus appropriate to first assess whether the stability range of the 冑5 surface oxide does, indeed, extend to the catalytically relevant environments when the kinetics of the ongoing CO2 formation is fully accounted for. In this study, we determine this stability range by focusing on the onset of the decomposition of the surface oxide structure when the partial pressure ratio pCO : pO2 exceeds a critical value. We identify this onset once the average O concentration in the 冑5 structure is reduced below the value corresponding to the intact surface oxide, which allows us to restrict our kMC modeling to the 冑5 lattice. The central result of our kMC simulations, which we had briefly highlighted before,14 is that at ambient pressures the surface oxide is stabilized at the surface up to CO : O2 partial pressure ratios just around the catalytically most relevant stoichiometric feeds 共pCO : pO2 = 2 : 1兲. This suggests an interpretation of the morphological changes observed in recent reactor scanning-tunneling microscopy 共STM兲 measurements15 under O-rich feeds in terms of a formation of the 冑5 structure at the surface. Furthermore, the precise value for the critical partial pressure ratio we compute sensitively depends on temperature, so that both local pressure and temperature fluctuations may induce a continuous formation and decomposition of the oxidic phase during steadystate operation under ambient stoichiometric conditions. We therefore expect that a full understanding of the catalytic 155410-1 ©2008 The American Physical Society PHYSICAL REVIEW B 77, 155410 共2008兲 ROGAL, REUTER, AND SCHEFFLER activity of the Pd共100兲 surface in such technologically relevant environments can only be obtained from a modeling that explicitly accounts for the corresponding ongoing structural changes, which will then also be able to address the actual role played by the surface oxide for the catalytic activity itself. Nevertheless, the rather high peak turnover frequencies obtained in our simulations even at the intact surface oxide show already that the formation of this structure in the reactive environment cannot simplistically be equated to a “deactivation” of the model catalyst. II. THEORY A. First-principles kinetic Monte Carlo simulations Our target is to describe the steady-state catalytic CO oxidation over the 冑5 surface oxide by explicitly accounting for the kinetics of the different elementary processes taking place in the system. Properly evaluating the time evolution of such a system requires simulation cells that are large enough to capture the effects of correlation and spatial distribution of the chemicals at the surface. Furthermore, most of the considered processes are highly activated and occur on time scales that are orders of magnitude longer than, e.g., a typical vibration 共⬃10−12 s兲. Due to these so-called rare events, we need to evaluate the statistical interplay between the different elementary processes over an extended time scale that can reach up to seconds or more. Since this is unfeasible for molecular dynamics simulations, we employ kinetic Monte Carlo simulations, where the time evolution is efficiently coarse grained to the rare-event dynamics. In a kMC simulation, each kMC step corresponds to the execution of a rare event, while appropriately accounting for the short-time dynamics of the system in between. In the generated sequence of system states, each state is assumed to be independent of all previous states, i.e., the kMC algorithm provides an efficient numerical solution to the master equation of a continuous time Markov process.16–20 In order to keep the number of considered elementary processes in a tractable range, the kMC simulations are performed on a lattice. Obviously, the chosen lattice model has to properly reflect the important structural features of the real system. For this model, a list of all relevant elementary processes p on the lattice is set up with the corresponding rate constants k p that characterize the probability to escape from the present system state by the process p. By starting in a given initial system configuration, the sum over the rate constants of all possible processes in this current configuration is evaluated, ktot = 兺 pk p. One process i is then randomly chosen by i−1 i 兺 kp ⬍ 1ktot 艋 p=0 兺 kp , 共1兲 p=0 with 1 苸 兴0 , 1兴 being a random number. Since the probability of selecting a process i is weighted by its rate constant ki, a process with a large rate constant is more likely to be chosen than a process with a small rate constant. The selected process is executed and the system configuration is updated. This way the kMC algorithm simulates a sequence of Poisson processes, and an explicit relationship between kMC time and real time can be established.20 This evolution of real time after each kMC step is given by t→t− ln共2兲 , ktot 共2兲 where 2 苸 兴0 , 1兴 is a second random number.20 The crucial ingredients to a meaningful kMC simulation are therefore the identification of all relevant elementary processes p and the determination of the corresponding rate constants k p. For the latter, we rely on the modern first-principles kinetic Monte Carlo approach21–28 and calculate the rate constants using DFT and transition-state theory 共TST兲. Concerning the elementary processes during the CO oxidation over the 冑5 surface oxide, we consider the adsorption, desorption, diffusion, and reaction of the chemicals, and follow the recipe of how to determine the rate constants for these processes from DFT and TST given in Ref. 28. In the next section, the resulting expressions for the rate constants are briefly reviewed. The first-principles data required to evaluate the rate constants with these expressions are then given in Sec. II E. B. Rate constants 1. Adsorption The rate constant of adsorption of a gas phase species i on a surface site of type st depends on the impingement rate and the local sticking coefficient S̃i,st as follows 共Ref. 28兲: ads 共T,pi兲 = S̃i,st共T兲 ki,st p iA 共3兲 冑2mikBT . The only system-specific parameters entering the impingement rate are the mass mi of the impinging gas phase molecules and the surface area A. An explicit accurate evaluation of the local sticking coefficient S̃i,st is highly involved and requires a determination of the full high-dimensional potential energy surface 共PES兲 of the adsorption process, on which molecular dynamics simulations have to be performed for a statistically relevant number of trajectories.29 In the present study, the local sticking coefficient is instead roughly estimated as28 ads S̃i,st共T兲 = f i,st 共T兲 冉 冊 冉 冊 ads ⌬Ei,st Ai,st exp − , A k BT 共4兲 ads is the highest barrier along the minimum energy where ⌬Ei,st pathway 共MEP兲 and Ai,st is the so-called active area. Within the concept of an active area, it is assumed that only particles of a species i with an initial lateral position within a certain area Ai,st around the adsorption site st can actually stick to this site. The rate constant of adsorption in Eq. 共3兲 will then actually become independent of the total impingement area ads is a A, and only the active area Ai,st has to be known. f i,st factor that reduces the number of impinging gas phase particles by the fraction that is not traveling along the MEP and might thus be reflected at some higher barrier along a different pathway. 155410-2 PHYSICAL REVIEW B 77, 155410 共2008兲 CO OXIDATION ON Pd共100兲 AT TECHNOLOGICALLY… 2. Desorption Since the desorption process is the time-reversed process of adsorption, the desorption rate constants are connected to the adsorption rate constants by a detailed balance criterion and can thus be obtained by applying28 冉 des ads ki,st = ki,st exp − ads ⬇ ki,st 1 vib zi,st ⌬Gi,st共T,pi兲 k BT 冉 冊 冊 bind ⌬i,gas共T,pi兲 − Ei,st exp − , k BT 共5兲 where ⌬Gi,st共T , pi兲 is the change in the Gibbs free energy between a particle in the gas phase and in the adsorbed state. ⌬Gi,st共T , pi兲 is approximated by the difference between the chemical potential of the particle in the gas phase, tot i,gas共T , pi兲 = Ei,gas + ⌬i,gas共T , pi兲 and the free energy of the tot vib − kBT ln共zi,st 兲. To particle in the adsorbed state, Fi,st = Ei,st evaluate the desorption rate constant using Eq. 共5兲, we thus need to determine, in addition to the adsorption rate constant, the vibrational partition function of the particle in the advib , the temperature and pressure dependent sorbed state, zi,st part of the gas phase chemical potential, ⌬i,gas共T , pi兲, as bind tot tot = Ei,gas − Ei,st , of the particle well as the binding energy, Ei,st at its adsorption site st. 3. Diffusion In a diffusion process, a particle i moves from a site st to a site st⬘. If an appropriate saddle point along the diffusion pathway can be identified, harmonic TST can be applied to obtain the corresponding rate constant of diffusion28 diff ki,st→st⬘共T兲 = diff,TST f i,st→st⬘ 共T兲 冉 冊 冉 diff 冊 ⌬Ei,st→st⬘ k BT exp − , h k BT 共6兲 with vib diff,TST f i,st→st⬘ 共T兲 = zi,st→st⬘,TS vib zi,st 共7兲 and diff tot tot . ⌬Ei,st→st⬘ = Ei,st→st⬘,TS − Ei,st 共8兲 diff denotes the maximum barThe diffusion barrier ⌬Ei,st→st ⬘ rier along the MEP of the diffusion process and is given by tot the energy difference of the transition state 共Ei,st→st 兲 and ⬘,TS tot the initial state 共Ei,st兲 at site st. The reverse process of the diffusion st→ st⬘ is simply the backward diffusion st⬘ → st and, therefore, the rate constants of these two processes have to fulfill the detailed balance criterion. To calculate the difdiff,TST fusion rate constants, the factor f i,st→st 共given by the ratio of ⬘ vib , and the vibrational partition functions in the TS, zi,st→st ⬘,TS vib 兲 as well as the diffusion barriers have to the initial state zi,st be known. 4. Reaction If a suitable reaction coordinate can be identified that contains a saddle point, again TST can be used to determine the reaction rate constant. In a general form, the reaction rate constant can then be written as28 reac,TST kreac 共T兲 i→f 共T兲 = f i→f 冉 冊 冉 冊 reac ⌬Ei→f k BT exp − , h k BT 共9兲 with i denoting the initial state and f the final state of the reaction process. As for the diffusion events, the factor reac,TST can be obtained from the ratio of the partition funcf i→f tions in the transition and initial states. In addition, the reaction barrier, ⌬Ereac i→f , defined as the energy difference in the transition and initial state, has to be determined. C. Computational setup The most crucial input parameters to determine the rate constants as discussed in the previous section are the energy barriers for adsorption, diffusion, and reaction, as well as the binding energies at a certain adsorption site. We calculate the total energies that are needed to evaluate these quantities using DFT and within the full-potential 共linearized兲 augmented plane orbital 共L兲APW+lo method30,31 as implemented in the WIEN2K code.32 The exchange-correlation 共xc兲 energy is treated within the generalized gradient approximation using the Perdew–Burke–Ernzerhof33 xc functional. All surfaces are simulated by using the supercell approach with inversion symmetric slabs consisting of five Pd共100兲 layers with the reconstructed surface oxide layer plus additional O / CO on both sides. We verified that further increasing the number of Pd共100兲 layers to 7 changes the binding energies of both adsorbates by an insignificant amount 共艋2 meV per adsorbate兲. The vacuum between consecutive slabs is at least 14 Å. The outermost adsorbate layers, the surface oxide and topmost palladium substrate layer, are fully relaxed. All of the calculations of gas-phase molecules 共O, CO, and CO2兲 are done in rectangular supercells with side lengths of 共13 ⫻ 14⫻ 15兲 bohr 共for O兲, 共13⫻ 14⫻ 18兲 bohr 共for O2 and CO兲, and 共13⫻ 14⫻ 20兲 bohr 共for CO2兲. Pd = 2.0 bohr for pallaThe muffin-tin radii are set to RMT O C = 1.0 bohr for cardium, RMT = 1.0 bohr for oxygen, and RMT bon. Inside the muffin tins, the wave functions are expanded wf pot = 12 and the potential up to lmax = 6. For the 冑5 up to lmax surface unit cell, a 关4 ⫻ 4 ⫻ 1兴 Monkhorst–Pack 共MP兲 grid 共eight irreducible k points兲 has been used to integrate the Brillouin zone 共BZ兲 and, for larger surface unit cells, the MP grid has been reduced accordingly to assure an equivalent sampling of the BZ. For the gas-phase molecule calculations in the large rectangular supercells, ⌫-point sampling was employed. The energy cutoff for the expansion of the wave wf = 20 Ry and, for the potenfunction in the interstitial is Emax pot tial, Emax = 196 Ry. The chosen computational setup is thus exactly the same as in the preceding thermodynamic study on this system.6 As detailed there6 using these basis set parameters, the reported binding energies per oxygen atom or per CO molecule are converged to within 50 meV, which is fully sufficient for the arguments and conclusions presented here. 155410-3 PHYSICAL REVIEW B 77, 155410 共2008兲 ROGAL, REUTER, AND SCHEFFLER D. Kinetic Monte Carlo model Having established the theoretical framework for the kMC simulations, the next crucial step is to build a suitable lattice model that represents the investigated system. For this, we use the insight gained in our preceding constrained thermodynamics study6 that identified the 冑5 as the most relevant oxidic structure under catalytically interesting gasphase conditions 共pi ⬃ 1 bar, T ⬃ 300– 600 K兲. As initially discussed in Sec. I, we thus concentrate the kMC simulations on this particular structure and develop a first-principles kMC lattice model that allows for a proper mapping of the 冑5 surface oxide structure. ( 5 5 ) R 27 Pd(100) 1. Kinetic Monte Carlo lattice In the upper panel of Fig. 1, a schematic illustration of the surface oxide on Pd共100兲 is shown. The 冑5 surface oxide structure characterized in UHV essentially corresponds to a 共O-Pd-O兲 trilayer of PdO共101兲 on top of the Pd共100兲 substrate.12 Each 冑5 surface unit cell contains four Pd atoms in the reconstructed oxide layer. In this stoichiometric termination of the surface oxide, two of the Pd atoms are fourfold coordinated and two are twofold coordinated by oxygen. There are also two kinds of oxygen atoms, two of them sit on top of the reconstructed Pd layer 共upper O atoms兲 and two at the interface to the Pd共100兲 substrate 共lower O atoms兲, forming the previously mentioned trilayer structure. At first sight, the surface oxide structure exhibits six highsymmetry adsorption sites within the 冑5 surface unit cell, where either oxygen or CO can be adsorbed.6 These are two bridge sites 共br兲, two twofold by oxygen coordinated top sites 共top2f兲, and two fourfold by oxygen coordinated top sites 共top4f兲. The difference between each of these doubly existing adsorption sites arises only from the arrangement of the underlying Pd共100兲 lattice. These small structural deviations seem to have little consequences on the binding at these different prominent adsorption sites. The computed binding energies of O and CO in the two bridge sites differ by less than 0.1 eV. Similarly, for the two top2f and top4f sites, the difference is even smaller, ⌬Ebind ⬍ 50 meV 共a more detailed discussion of the binding energetics can be found in Ref. 6兲. In our kMC model, we therefore neglect these small differences and build the lattice from the half sized 冑5 surface unit cell as shown in Fig. 1, each containing three different adsorption sites, bridge, twofold top, and fourfold top. Inspecting the computed energetics at these three different adsorption sites in more detail, the kMC lattice model can even be further simplified. We find that in the top2f and top4f sites, the CO is bound much weaker, i.e., by 0.3– 0.8 eV, as compared to the bridge site. In addition, the two top sites correspond only to very shallow PES minima, with diffusion barriers of less than 50 meV to a neighboring bridge site. Considering further that due to the computed strongly repulsive interactions6 it is not possible to adsorb CO at a top site next to an already occupied bridge site, we realize that the metastable top sites will effectively never be occupied. For oxygen, the situation is even more pronounced, since here the additional adsorption of an O atom at the 冑5 surface oxide is only possible in the bridge site, whereas the two top ( 5 5 ) R 27 FIG. 1. 共Color online兲 In the upper panel, a schematic top view of the 冑5 surface oxide structure is shown. The large gray spheres represent Pd atoms, the small red 共dark兲 ones O atoms. The Pd atoms of the Pd共100兲 substrate are darkened. The 冑5 surface unit cell as well as the 共1 ⫻ 1兲 surface unit cell of Pd共100兲 are indicated. As illustrated, the 冑5 surface unit cell consists of two halves that differ only with respect to the underlying Pd共100兲 substrate. We find the difference in binding energies at the equivalent adsorption sites in the two halves to be very small and, correspondingly, use the reduced unit cell in the kMC simulations. In the lower panel, these prominent adsorption sites and the final kMC lattice are illustrated. The three high-symmetry adsorption sites 共bridge, top2f, and top4f兲 are indicated by the yellow 共light兲 crosses. The hollow adsorption site of the upper O atoms 关red 共dark兲 cross兴 is likewise included as a site in the kMC lattice, whereas the reconstructed Pd layer as well as the lower O atoms are fixed. In the final kMC lattice, only the bridge and hollow sites are considered, as shown on the lower left 共see text兲. sites are not even metastable. The two different top sites are therefore disregarded in setting up the kMC lattice representation of the surface oxide. On the other hand, considering only the adsorption into prominent high-symmetry sites at the perfect 冑5 structure is not sufficient to address the CO-induced decomposition of this lattice. For this, we assume that the surface oxide layer starts to destabilize by the removal of the upper oxygen atoms from the trilayer structure. We therefore also include the corresponding hollow sites that are completely occupied by these surface oxygen atoms in the perfectly stoichiometric 冑5 structure as explicit sites in the kMC model 共cf. Fig. 1兲. The basis for the final kMC lattice model is thus formed by the fixed reconstructed Pd layer and the lower O atom in the PdO trilayer. On this lattice, there are two different active 155410-4 PHYSICAL REVIEW B 77, 155410 共2008兲 CO OXIDATION ON Pd共100兲 AT TECHNOLOGICALLY… site types 共br and hol, cf. left part of the lower panel in Fig. 1兲. Each site can either be vacant or filled with one oxygen atom or one CO molecule, whereas multiple adsorption at a site is not possible. Considering all nonconcerted processes possible on this lattice, we obtain a total number of 26 possible processes. This includes five adsorption processes, the unimolecular adsorption of CO into br or hol sites and the dissociative adsorption of O2 into adjacent br-br, br-hol, or hol-hol sites, as well as the corresponding five desorption processes. Furthermore, there are eight site- and element-specific diffusion processes describing the diffusion of O / CO from br→ br, hol → hol, br→ hol, and hol→ br sites, as well as four reaction processes including the reaction of Obr + CObr, Ohol + COhol, Obr + COhol, and Ohol + CObr. Since the reaction processes are modeled as associative desorption, there are four additional processes for the dissociative adsorption of CO2. This list of nonconcerted processes is exhaustive with respect to the chosen kMC lattice setup. However, it cannot be excluded that there might also be other more complex concerted processes that could have an influence on the system discussed here. 2. Simulation setup All kMC simulations are performed on the final lattice model containing 共10⫻ 10兲 half 冑5 surface unit cells, i.e., 100 br and 100 hol sites, with periodic boundary conditions. To ensure that the size of the chosen lattice is sufficient, simulations were also performed on larger lattices containing up to 1250 bridge and hollow sites, respectively, without observing significant differences concerning the investigated quantities. These quantities of interest for the present study are the average surface occupations ¯i,st of a particle i on a site st under steady-state conditions, which are evaluated as ¯ = 兺ni,st,n · ⌬tn , i,st 兺n⌬tn 共10兲 where ⌬tn is the time step of the nth Monte Carlo move. In all of the simulations, we checked carefully, by using different starting configurations and varying simulation lengths, that the system actually reached steady state before the average surface occupations were evaluated. E. Evaluation of the rate constants For all of the 26 processes that are possible in the kMC model, the rate constants have to be determined. The respective expressions for the four different process types, i.e., adsorption, desorption, diffusion, and reaction, have been described in Sec. II B. Here, we determine the corresponding parameters entering the equations for the different rate constants following the procedure described in more detail in Ref. 28. 1. Adsorption To calculate the rate constants of adsorption in Eq. 共3兲, we specify the active area Ai,st for the impingement of each species on each site as simply half the surface area of the surface unit cell in the kMC lattice. As shown in Fig. 1, this area corresponds to half the surface unit cell of the 冑5 structure 共1 / 2A冑5 = 19.47 Å2兲, i.e., ACO,br = ACO,hol = 1 / 4A冑5 for the adsorption of CO and AO2,br-br = AO2,hol-hol = AO2,br-hol = 1 / 6A冑5 for the adsorption of O2. To obtain an estimate for the local sticking coefficient S̃i,st in Eq. 共4兲, we perform DFT calculations to determine first of ads , along the MEP all if there are any significant barriers, ⌬Ei,st for any of the five different adsorption processes. For the CO molecule, this was done by vertically lifting the CO in an upright geometry from a bridge 共hollow兲 site. For different heights of the CO molecule, above its adsorption site, the energy of the whole system was then minimized with respect to all other degrees of freedom. For neither of the two sites a barrier was found along this desorption 共adsorption兲 pathads ads = ⌬ECO,hol = 0.0 eV. For the dissociative adway, i.e., ⌬ECO,br sorption of O2 molecules, a PES was mapped out, in which the energy is given as a function of the bond length between the two O atoms and the height above the surface of their center of mass 共so-called elbow plot兲. The lateral position of the center of mass within the surface unit cell as well as the orientation of the O2 molecule were kept fixed. Since there are only two hollow sites within the 冑5 surface unit cell, a lifting of two oxygen atoms would correspond to a complete removal of all upper oxygen atoms in the surface oxide structure due to the periodic supercell setup of the DFT calculations. Therefore, for these calculations, the size of the 冑5 surface unit cell was doubled in the direction of the involved sites. We find that the dissociation of an O2 molecule in this particular orientation appears to be nonactivated. A similar result is also found for the O2 adsorption in neighboring ads ads = ⌬EO = 0.0 eV. For bridge-hollow sites, i.e., ⌬EO 2,hol-hol 2,br-hol the adsorption in two neighboring bridge sites, though, the ads = 1.9 eV. PES reveals a high barrier of ⌬EO 2,br-br A second parameter entering the sticking coefficient in ads representing the reduction in sticking Eq. 共4兲 is the factor f i,st due to the fraction of impinging molecules not following the MEP. Since the kMC simulations are performed in a temperature range of T = 300– 600 K, where the impinging gasphase molecules can still be considered as rather slow, it is assumed that the molecules are quite efficiently steered along ads is approximated by the MEP and, thus, the value of f i,st ads f i,st ⬇ 1 for all five adsorption processes. With these parameters, the sticking coefficients are unity for the four barrierfree adsorption processes. For the activated adsorption of O2 on two neighboring bridge sites, the sticking coefficient is as small as ⬃10−16 even for a temperature of T = 600 K. Even if the crude way of extracting the approximate activation barrier from the restricted elbow plot would thus introduce an error of many orders of magnitude in the sticking coefficient, this adsorption process will therefore still be insignificant as compared to the adsorption of O2 in two neighboring hollow or neighboring bridge and hollow sites. The results of the kMC simulations reported below where, indeed, found to be unaffected, even when lowering the activation barrier for this adsorption process by up to 0.5 eV. 2. Desorption Having determined the five different adsorption rate constants, the respective desorption rate constants can be calcu- 155410-5 PHYSICAL REVIEW B 77, 155410 共2008兲 ROGAL, REUTER, AND SCHEFFLER lated using detailed balance via Eq. 共5兲. To a first approximation, the vibrational partition function in the adsorbed vib ⬇ 1, for all five state entering Eq. 共5兲 is set to unity, zi,st desorption processes. In the gas phase, this approximation would certainly be reasonable over the temperature range 共T = 300– 600 K兲 investigated here, i.e., only the first vibrational state of the O2 and CO molecules is excited. In the adsorbed state, though, this might be changed due to the lower frequency modes resulting from the adsorbatesubstrate bond, which could then lead to a somewhat larger vib ⬎ 1, and therefore slightly smaller departition function, zi,st sorption rate constants. Since this enters only linearly into the desorption rate constant, we, nevertheless, found that considering such increased partition functions did not significantly affect the conclusions drawn from the simulations below. The temperature and pressure dependent part of the gasphase chemical potential ⌬i,gas共T , pi兲 is calculated by approximating the O2 and CO gas phase with ideal gas-phase reservoirs and evaluating the translational, vibrational, rotational, electronic, and nuclear partition functions using statistical thermodynamics.34 This approximation by an ideal gas only introduces a negligible error in the temperature and pressure range considered here.34 A further parameter that is needed to evaluate Eq. 共5兲 is the binding energy of the particles in their respective adsorpbind . Since the binding energies of O and CO in tion sites, Ei,st bridge and hollow sites also depend on lateral interactions between the adsorbates, we expand them in a lattice gas Hamiltonian 共LGH兲.35–39 Aiming only at a first approximation of the effect of lateral interactions, we employ a crude LGH that is restricted to the nearest neighbor pair interactions between adsorbates in different and alike sites, yielding 0 0 + nCO,iECO,i 兴 + 兺 关VO-O,ij nO,i nO,j H = 兺 关nO,iEO,i i ij + VCO-CO,ij nCO,i nCO,j + VO-CO,ij nO,i nCO,j兴, 共11兲 where i runs over all lattice sites in the kMC lattice and j 0 only over the corresponding nearest neighboring sites. EO,i 0 and ECO,i are the on-site energies of O and CO on a site i, Vi,j is the interaction parameter between two adsorbates sitting on sites i and j, and ni is the occupation number, i.e., ni = 0 denotes that site i is empty and ni = 1 denotes that it is occupied. To obtain an estimate of the error introduced by limiting the LGH to the nearest neighbor pair interactions only, we performed DFT calculations with sparser adsorbate arrangements in larger surface unit cells, i.e., in 共2冑5 ⫻ 冑5兲R27° and 共冑5 ⫻ 2冑5兲R27° cells. The obtained binding energies of O and CO in these larger surface unit cells differ by less than 0.1 eV from the respective values calculated within the 冑5 surface unit cell. This change in binding energies is within the level of accuracy assumed here, rationalizing the choice to neglect lateral interactions between adsorbates extending beyond the 冑5 surface unit cell in the current study. Employing the LGH in Eq. 共11兲, the binding energy of a CO molecule in a site i is then given by Vbr-br Vhol-hol Vbr-hol FIG. 2. 共Color online兲 Considered nearest neighbor pair interactions between adsorbates on the 冑5 surface oxide lattice. Large gray spheres represent Pd atoms. Small red spheres represent oxygen atoms included in the kMC lattice. Small yellow spheres represent adsorbed O and/or CO. bind ECO,i = H共nCO,i = 1兲 − H共nCO,i = 0兲 0 = ECO,i + 2 兺 关VCO-CO,ijnCO,j + VO−CO,ijnO,j兴. j 共12兲 Accordingly, the binding energy of an oxygen atom is calculated. During the associative desorption of an O2 molecule, respectively, two neighboring sites are depleted, which can be expressed likewise using the LGH. As shown in Fig. 2, the first nearest neighbor pair interactions correspond to interactions between two neighboring bridge sites, between two neighboring hollow sites, and between neighboring bridge and hollow sites. This generates six different interaction parameters between like species 共VO-O,br-br, VO-O,hol-hol, VO-O,br-hol, VCO-CO,br-br, VCO-CO,hol-hol, and VCO-CO,br-hol兲 and four different ones between unlike species 共VO-CO,br-br, VO-CO,hol-hol, VO-CO,br-hol, and VO-CO,hol-br兲. Together with the four on-site energies, we thus have to determine 14 parameters for the LGH. This is achieved by fitting the parameters to DFT total energies of 29 different ordered configurations with O and/or CO in bridge and hollow sites within the 冑5 surface unit cell, and by expressing the respective energy of each configuration in terms of the LGH expansion 关cf. Eq. 共11兲兴. Since within the kMC model the lower oxygen atoms of the 冑5 surface oxide trilayer form a part of the lattice itself, the energies of the different configurations are calculated with respect to the empty kMC lattice, i.e., tot ⌬E共O,[email protected]冑5 − 2O兲 = EO,[email protected]冑5−2O − E冑5−2O − NO1/2EO 2 tot − NCOECO , 共13兲 where E冑5−2O corresponds to the total energy of the surface oxide structure without the two upper oxygen atoms. The tot , is calculated by total energy of an oxygen molecule, EO 2 tot tot bind using the relationship EO = 2EO + EO with a highly con2 2 verged value of the oxygen gas-phase binding energy of bind = −6.22 eV.40 Table I lists the determined values for the EO 2 four on-site energies and ten interaction parameters. With these parameters, the binding energy of every adsorbate for any random configuration on the lattice can be evaluated by using Eq. 共12兲. With this binding energy, the respective desorption rate constants can then be calculated via Eq. 共5兲. 155410-6 PHYSICAL REVIEW B 77, 155410 共2008兲 CO OXIDATION ON Pd共100兲 AT TECHNOLOGICALLY… TABLE I. Four on-site energies E0 and ten first nearest neighbor pair interaction parameters V for the lattice gas Hamiltonian describing the adsorption of O and CO in hollow and bridge sites on the 冑5 surface oxide. All values are in eV. TS ∆ Ediff TS final 0 EO,br 0 EO,hol 0 ECO,br 0 ECO,hol −0.51 −1.95 −1.40 −1.92 VO-O,br-br 0.08 VO-O,hol-hol 0.07 VO-O,br-hol 0.08 VCO-CO,br-br 0.08 VCO-CO,hol-hol 0.13 VCO-CO,br-hol 0.14 VO-CO,br-br 0.06 VO-CO,hol-hol 0.11 VO-CO,br-hol 0.13 ∆ Ediff initial final initial FIG. 3. Schematic illustration of the diffusion barriers between energetically like and unlike sites. VO-CO,hol-br 0.12 3. Diffusion Within the kMC lattice model for the 冑5 surface oxide, there are eight different diffusion processes, four between like sites 共O / CO hol→ hol and br→ br兲 and four between unlike sites 共O / CO hol→ br and br→ hol兲. To obtain the corresponding rate constants of diffusion, the vibrational partition functions of the adsorbates in the initial state and in the transition state are needed, as well as the diffusion barriers 关cf. Eqs. 共6兲 and 共7兲兴. With a similar justification as for the desorption rate constants, we assume the partition functions in initial and tranvib vib ⬇ zi,st→st , yielding sition states to be comparable, i.e., zi,st ⬘,TS diff,TST f i,st→st⬘ ⬇ 1 for all eight diffusion processes. To calculate the diff , we determine the transition state diffusion barriers, ⌬Ei,st→st ⬘ by defining a reaction coordinate connecting the initial and final states and we calculate the energy of O / CO for different positions along this coordinate. Since we found the surface oxide trilayer to be rather mobile with respect to a registry shift parallel to the Pd共100兲 substrate,6 the lateral positions of the reconstructed Pd atoms are additionally kept fixed in these calculations. The resulting barriers for these approximate diffusion paths are listed in Table II. The barriers have been calculated within the 冑5 surface unit cell with both hollow sites occupied by O 共O / CO diffusion br→ br兲, only one hollow site occupied by O 共O / CO diffusion hol → br兲, and one hollow site occupied by either O or CO 共O / CO diffusion hol→ hol兲. The initial and final states of a diffusion process can either be energetically degenerate 共left part of Fig. 3兲 or—for the diffusion between unlike sites or like sites with a different nearest neighbor coordination—the energies of the initial and final state wells differ 共right part of Fig. 3兲. In the latter case, the values listed in Table II repreTABLE II. Barriers for the diffusion between the different sites within the 冑5 surface unit cell. All values are in eV. O CO ∆ Ebind diff ⌬Ebr→br ⌬Ediff hol→hol diff ⌬Ehol→br 1.2 0.4 1.4 0.6 0.1 0.3 sent the minimum value of the diffusion barrier, i.e., if the final state has the same or a lower energy than the initial state, the diffusion barrier is equal to the tabulated value. If, on the other hand, the final state is higher in energy, the difference in binding energies between the initial and final states is added to the listed barrier to ensure that the detailed balance criterion is fulfilled for the two time-reversed diffusion processes. Since this difference in binding energies depends on the nearest neighbor coordination of the two lattice sites involved in the diffusion process, lateral interaction effects are this way also considered in the diffusion process rate constants. The described approximations in determining the exact transition states lead to uncertainties in the stated barrier values, which, in turn, influence the corresponding diffusion rate constants. We checked on the importance of the various diffusion processes on the simulation results and found them to play only a minor role. Essentially, even completely switching off all diffusion processes led only to insignificant changes of the results presented below. We are thus confident that the rather coarse procedure to determine the diffusion barriers is sufficient with respect to the current purpose of the simulations. 4. Reaction To calculate the rate constants for the four possible reaction processes 共Obr + CObr, Ohol + COhol, Obr + COhol, and ⬇ 1 in Eq. 共9兲 is approximated Ohol + CObr兲, the factor f reac,TST i→f by unity. Again, it is thus assumed that, to a first approximation, the partition functions of the initial and transition states are in the same order of magnitude and, thus, the ratio of the two is close to 1. To determine the reaction barriers, ⌬Ereac i→f , the corresponding transition states are located by dragging the two reactants toward each other and mapping out the corresponding twodimensional PES 共Obr + COhol and Ohol + CObr兲. Hereby, only the coordinates of the reactants along the dragging direction are kept fixed, whereas all other coordinates are fully relaxed. Similar to the problem encountered when determining the diffusion barriers, the reconstructed palladium layer showed a rather high mobility with respect to a lateral shift along the substrate following the dragging direction. To circumvent this problem, a two-step approach was chosen to, nevertheless, identify appropriate transition states. In the first step, the lateral coordinates of the reconstructed palladium layer were additionally fixed and the energy is only minimized with respect to the remaining coordinates. In a second step, the identified transition state geometry is relaxed with 155410-7 PHYSICAL REVIEW B 77, 155410 共2008兲 ROGAL, REUTER, AND SCHEFFLER TABLE III. Barriers for the reaction of O and CO adsorbed in different sites within the 冑5 surface unit cell. All values are in eV. br O + CO ⌬Ereac 1.0 br O hol + CO hol br O + CO 1.6 0.5 hol O hol + CO 600 K 300 K br 0.9 300 K 400 K respect to the lateral coordinates of the topmost Pd layer while fixing the coordinates of the reactants O and CO to release some of the lateral stress that was induced by fixing the lateral positions of the Pd atoms in the first step. For the reaction of Obr + CObr and Ohol + COhol, this two-step approach was not necessary. Similar to the dissociative adsorption of O2, an elbow plot was calculated, giving the energy as a function of the O-CO distance and the height of the corresponding center of mass above the surface. Due to the symmetry of the calculated geometries, no shift of the substrate layer could occur in this case. All correspondingly calculated reaction barriers are summarized in Table III. For the reaction processes, the energies of the initial, transition, and final states are also influenced by the nearest neighbor interactions. By inspecting the geometries of the transition states, they appear to be more related to the initial states and, therefore, we assume that the transition states are similarly affected by these interactions as the initial states. Thus, the energy difference between the initial and transition states is not influenced by the nearest neighbor interactions and the reaction barriers are constant with respect to different configurations on the surface. Since the reaction processes are modeled as associative desorption, the corresponding time-reversed process is the dissociative adsorption of CO2 into the respective sites. The adsorption barrier for such a process can be obtained from the reaction barrier and the corresponding binding energies of O and CO on the surface with respect to the free CO2 molecule. The lowest of the four resulting barriers for the dissociative adsorption of CO2 共leading to a CO in a bridge site and O in a neighboring hollow site兲 is still very large, ads with ⌬ECO ,br-hol = 1.4 eV. At a temperature of T = 600 K, the 2 local sticking coefficient S̃CO2,br-hol is, even in this case, only of the order of 10−12. Even if the CO2 generated at the surface is not readily transported away and a noticeable CO2 pressure would build up close to the surface, the readsorption of CO2 on the surface is therefore still negligible due to the very low sticking coefficient and, thus, is not explicitly considered in the kMC simulations. III. RESULTS Having established the setup of the kMC lattice model and the respective rate constants for the 26 different processes based on DFT energetics and harmonic TST, we proceed to the results of the kMC simulations. Since the kMC simulations are performed in an open system with a continuous supply of reactants and removal of products, we are describing an intrinsically nonequilibrium system. In the following, we will refer to a state of constant average surface occupations at steady state over a range of 600 K FIG. 4. 共Color online兲 Thermodynamic surface ‘‘phase’’ diagram of the Pd共100兲 surface in a constrained equilibrium with O2 and CO gas phase as described in detail in Ref. 6. The differently shaded areas mark the stability regions of various surface structures for a given chemical potential of the O2 and the CO gas phase. Blue 共solid兲 areas include O / CO adsorption structures on Pd共100兲, red and white 共hatched兲 areas comprise surface oxide structures, and the gray 共crosshatched兲 area represents the stability range of bulk PdO. For convenience, the dependence of the chemical potential of the two gas phases is translated into pressure scales for T = 300 K and T = 600 K 共upper x axes and right y axes兲. For the stability region of the surface oxide structures, additional schematic figures of the different surface configurations are shown. Large gray spheres represent Pd atoms, small red 共dark兲 spheres represent oxygen atoms, and small yellow 共light兲 spheres represent CO molecules. The white arrows indicate the pressure conditions of the kMC simulations for temperatures of T = 300 K, T = 400 K, and T = 600 K. The oxygen pressure is always fixed at pO2 = 1 atm, while the CO pressure is varied between 10−5 艋 pCO 艋 105 atm. temperature and pressure conditions as “phases” in analogy to a phase in a closed thermodynamic system. In accordance with Ziff et al.,41 changes in these average surface occupations due to changes in temperature and pressure are then described in terms of “kinetic phase transitions.” Although the established kMC model has a wider range of applicability, we focus here on the stability of the thin surface oxide layer during steady-state catalytic CO oxidation at the surface. A. Reproducing the thermodynamic ‘‘phase’’ diagram In order to make contact to our preceding constrained thermodynamics work,6 we perform the kMC simulations in a first step only considering adsorption, desorption, and diffusion processes, whereas the reaction processes are excluded. The occupation of the different sites at the surface under steady-state conditions reflects then the same situation as a surface in a constrained thermodynamic equilibrium with an oxygen and CO gas phase, but including the effect of configurational entropy.5 The results of the constrained thermodynamics approach are summarized in Fig. 4 共for a detailed discussion, see Ref. 6兲. In the shown ‘‘phase’’ diagram, the most stable surface structures for any given chemical potential of the O2 and CO gas phase are presented 共the 155410-8 PHYSICAL REVIEW B 77, 155410 共2008兲 CO OXIDATION ON Pd共100兲 AT TECHNOLOGICALLY… respective pressure scales for T = 300 and 600 K are given in the upper x axes and right y axes兲. The stability regions of the different surface structures are denoted by differently shaded areas and, due to the neglected configurational entropy, the transitions between these stability regions are infinitely sharp.5,6 For the kMC simulations discussed here, it is particularly important that the different ‘‘phases’’ can be subdivided into three groups. All areas colored in blue 共solid兲 represent structures with O and CO adsorbed on the pristine Pd共100兲 surface; all red and white 共hatched兲 areas comprise structures involving the reconstructed 冑5 surface oxide; and the gray 共crosshatched兲 area marks the stability region of the bulk oxide. As discussed in Sec. II D, the kMC lattice model chosen here is based on the lattice structure of the 冑5 surface oxide and, therefore, does not allow for changes between this structure and the Pd共100兲 surface or the bulk oxide. Consequently, the constrained kMC simulations can only reproduce the part of the ‘‘phase’’ diagram where structures based on the surface oxide are most stable, i.e., the red/white-hatched region in Fig. 4. Within the constrained kMC simulations, we now evaluate the steady-state average occupation of bridge and hollow sites and compare the obtained structures to the structures predicted within the thermodynamic surface ‘‘phase’’ diagram. As mentioned above, the two approaches should yield equivalent results, except at the ‘‘phase’’ boundaries where configurational entropy is expected to become important.5 The simulations are performed for 共T , p兲 conditions that cover the entire stability region of the surface oxide 共red/ white- hatched兲 region in Fig. 4兴. Specifically, this means for T = 300 K, pressures of pO2 = 10−10 – 1010 atm and pCO = 10−10 – 1 atm, and for T = 600 K, pressures of pO2 = 1 – 1010 atm and pCO = 1 – 106 atm, respectively. We find that the kMC simulations accurately reproduce all four different surface oxide ‘‘phases’’ that appear in this part of the constrained ‘‘phase’’ diagram. In all four ‘‘phases,’’ all hollow sites are always filled with oxygen. The bridge sites are either empty, half filled with O or CO, or completely filled with CO depending on the respective gas-phase conditions and as detailed by the schematic representations in Fig. 4. As expected from the common underlying DFT energetics, we therefore find the results of the constrained kMC simulations to be fully consistent with those previously obtained within the constrained thermodynamics approach. The more extended sampling of configurations due to the LGH expansion within the kMC simulations does not lead to the appearance of new, stable ordered structures in the constrained ‘‘phase’’ diagram and, thus, confirms that the relevant configurations were included in the preceding thermodynamic approach. The effect of configurational entropy in the constrained kMC simulations is thus verified to “only” smear out the transitions between the different ordered ‘‘phases’’ at the finite temperatures considered,5 but does not affect the location of the ‘‘phase’’ boundaries themselves. Due to the hereby confirmed consistency between the two approaches, we can directly compare the results in the next section when allowing the reaction events to occur in the kMC simulation. This brings us in the position to directly address the effect of the kinetics of the ongoing chemical reactions on the surface structure and composition. B. Onset of surface oxide decomposition under reaction conditions By allowing the four different reaction processes to occur in the kMC simulations, we now proceed to evaluate the stability of the surface oxide structure under reaction conditions. Since the kMC lattice is fixed to the structure of the 冑5 surface oxide, the explicit structural change corresponding to the transition from the surface oxide to a pristine Pd共100兲 surface as predicted in the thermodynamic ‘‘phase’’ diagram 共red/white-hatched areas→ blue solid areas in Fig. 4兲 cannot directly be addressed. Instead, we start our simulations always in a 共T , p兲 range where the surface oxide is definitely the most stable ‘‘phase’’ 共high oxygen and low CO chemical potential兲 and where our kMC lattice model is certainly valid. By keeping the oxygen pressure and the temperature fixed, we then increase the CO pressure as indicated by the white vertical arrows in Fig. 4. Exceeding a certain pressure ratio of pO2 / pCO, we expect the onset of the decomposition of the 冑5 structure to be characterized by a depletion of the otherwise always essentially fully with oxygen occupied hollow sites. In the kMC simulations, we therefore monitor the average occupation of hollow sites by oxygen atoms, ¯Ohol, during steady state. If all hollow sites are occupied by oxygen, i.e., ¯Ohol ⬇ 100%, then the overall surface composition clearly represents the intact surface oxide structure 共this is the case in all four ‘‘phases’’ of the surface oxide structure in Fig. 4兲. If, on the other hand, at increasing pCO oxygen atoms get increasingly depleted beyond the amount of thermal fluctuations that create isolated, uncorrelated vacancies or double vacancies due to oxidation reaction or oxygen desorption events, then the deficiency of O atoms at the surface might destabilize the 冑5 surface structure and lead to a local lifting of the surface oxide reconstruction. Here, we therefore interpret a drop of the average occupation below 90% as the onset of a destabilization of the surface oxide. Since the average occupation is a global measure over the whole simulation cell, this quantity would be a bad indicator if there was an appreciable effective attraction between formed O vacancies. A decrease in the average occupation of hollow sites by oxygen of 10% could then involve a complete local depletion of 10% of the surface oxide area. In our kMC simulations, such a locally concentrated depletion of oxygen atoms is not observed. Instead, we find the formed oxygen vacancies to be distributed over the entire simulation cell and are thus confident that monitoring the average occupation, ¯Ohol, is a suitable measure to determine the onset of surface oxide decomposition. In this respect, the chosen drop to 90% is a conservative upper limit. As will become clear below, our conclusions are not affected by this specific choice and even the quantitative numbers for the transition pressures would vary only little if a drop to, say, 80% or 70% was chosen. The simulations are performed for three different temperatures, T = 300, 400, and 600 K. For each temperature, the oxygen pressure is fixed to pO2 = 1 atm and the simulations are run for different CO pressures in the range pCO = 10−5 – 105 atm covering the gas-phase conditions marked by the white arrows in Fig. 4. In Fig. 5, the corresponding simulation results are summarized. The steady-state average 155410-9 PHYSICAL REVIEW B 77, 155410 共2008兲 ROGAL, REUTER, AND SCHEFFLER Coverage θOhol (%) (a) 300K 100 80 60 40 20 0 -5 10 reac ∆EOhol+CObr = 0.9 eV reac ∆EOhol+CObr = 0.8 eV 0 10 CO pressure (atm) Coverage θOhol (%) (b) 5 10 400K 100 80 60 40 20 0 -5 10 reac ∆EOhol+CObr = 0.9 eV reac ∆EOhol+CObr surface oxide Pd(100) + CO = 0.8 eV 0 10 CO pressure (atm) (c) Coverage θOhol (%) surface Pd(100) + CO oxide 5 10 600K 100 80 60 40 20 0 -5 10 reac ∆EOhol+CObr = 0.9 eV reac ∆EOhol+CObr = 0.8 eV surface oxide Pd(100) + CO 0 10 CO pressure (atm) 5 10 FIG. 5. 共Color online兲 Average occupation of hollow sites by oxygen vs CO pressure for T = 300 K, T = 400 K, and T = 600 K. The vertical black line marks the boundary between the surface oxide and a CO covered Pd共100兲 surface as determined within the constrained thermodynamics approach. The influence of the barrier for the Ohol + CObr reaction is illustrated by showing the kMC simulation results for two barrier values of 0.9 and 0.8 eV 共see text兲. occupation of hollow sites with oxygen, ¯Ohol, is plotted vs the CO pressure. The solid 共green兲 lines represent the results obtained by using the calculated reaction barriers as listed in Table III. As has been discussed in Sec. II, several partly crude approximations were employed in the determination of the individual rate constants entering the kMC simulations. Before we proceed to analyze the obtained simulation results, we therefore critically assess the propagation of these underlying approximations and uncertainties to the final kMC results. We checked on this error propagation by systematically varying the rate constants over several orders of magnitude 共corresponding to variations in the respective energetic barriers of ⫾0.2 eV兲 and each time monitoring the effect on the average occupation displayed in Fig. 5. In al- most all cases, variations of the rate constants had an insignificant effect, which, as already described, concerns particularly all diffusion processes. Only if the barrier for the reaction process of an oxygen in a hollow site with a CO in a neighboring bridge site is altered will a noticeable change in the average surface populations occur. To get an estimate for the corresponding uncertainties in our presented results, we therefore additionally include in Fig. 5 the results for simulations using a 0.1 eV lower barrier for this reaction reac process Ohol + CObr, i.e., ⌬EO hol+CObr = 0.8 eV, while all other barriers have been left unchanged 关dashed 共orange兲 lines兴. The differences between these results 关dashed 共orange兲 line兴 and the results for the unmodified barrier 关solid 共green兲 line兴 provide then an indication of the uncertainty underlying our approach. Discussing first the top graph in Fig. 5, it can be seen that for a temperature of T = 300 K and an oxygen pressure of pO2 = 1 atm, the surface oxide is clearly stabilized for CO pressures up to pCO ⬍ 10−1 atm, i.e., under such gas-phase conditions, ¯Ohol ⬎ 95%. If the CO pressure is further increased, the O population at hollow sites starts to decrease and, for CO pressures of pCO ⬎ 1 atm, the surface oxide is certainly completely destabilized 共¯Ohol ⬇ 0兲. For the slightly lower reaction barrier 关dashed 共orange兲 line兴, a steeper decrease in the oxygen population is found, and the surface oxide is stabilized for CO pressures of pCO ⬍ 10−2 atm. To compare these results to the ones obtained within the constrained thermodynamics approach, the stability region of the surface oxide as determined in the ‘‘phase’’ diagram in Fig. 4 is indicated by the vertical black lines in the three graphs of Fig. 5. By following the white arrow in the ‘‘phase’’ diagram in Fig. 4 for T = 300 K and pO2 = 1 atm, this boundary between the surface oxide structure and a CO covered Pd共100兲 surface is reached for a CO pressure of pCO ⬇ 2 atm. Within the constrained thermodynamics approach, the surface oxide will thus be stable for pCO ⱗ 2 atm, whereas for pCO ⲏ 2 atm, the CO covered Pd共100兲 surface is the most stable ‘‘phase.’’ By comparing this to the kMC simulations, which include the effect of the CO2 formation kinetics, we see that the depletion of oxygen atoms in hollow sites and, thus, the destabilization of the surface oxide structure starts already at slightly lower CO pressures as compared to the transition from the stability region of the surface oxide to that of a CO covered Pd共100兲 surface in the ‘‘phase’’ diagram. Although we find the kMC simulations to be dominated by adsorption or desorption processes of the reactants 共as anticipated in the constrained thermodynamic approach assuming equilibrium with the gas-phase reservoirs兲, the kinetics of the ongoing oxidation reaction thus still leads to a slight decrease in the stability of the surface oxide. In turn, the kMC simulations predict that at a temperature of T = 300 K, oxygen-rich conditions 共pCO / pO2 ⬇ 1 : 10兲 are needed to stabilize the surface oxide structure. In Fig. 5共b兲, corresponding results are shown for T = 400 K. As compared to the simulations at T = 300 K, much more reaction processes take place in the kMC simulations at this higher temperature. For CO pressures of pCO ⬎ 10 atm, 155410-10 PHYSICAL REVIEW B 77, 155410 共2008兲 CO OXIDATION ON Pd共100兲 AT TECHNOLOGICALLY… though, almost no reaction processes are detected in the steady state, since under these conditions the surface is already completely filled with CO. Then again, this corresponds to gas-phase conditions where also in the constrained thermodynamics approach a CO covered Pd共100兲 surface is the most stable structure 共cf. Fig. 4兲. Similar to the results for T = 300 K, the surface oxide structure is completely stabilized for CO pressures of pCO ⬍ 10−1 atm. At a pressure ratio of pCO / pO2 = 2 : 1, i.e., here pCO = 2 atm, there are still 94% of all hollow sites occupied by oxygen 关solid 共green兲 line in Fig. 5共b兲兴. This result critically depends, however, on the barrier for the reaction of Ohol + CObr. If this barrier is decreased by only 0.1 eV, the occupation drops to 70% and, at reac ¯ an even lower barrier of ⌬EO hol+CObr = 0.7 eV, Ohol decreases even further to ⬃30% under these conditions. Whether or not the surface oxide prevails at this temperature for the catalytically most relevant stoichiometric partial pressure ratio can thus not be safely concluded in light of the uncertainties of our approach. For CO pressures lower than pCO ⬍ 10−1 atm, however, the surface oxide is definitely stabilized, just as much as it is definitely destabilized at CO pressures of pCO ⬎ 10 atm. We can therefore determine the onset of the surface oxide decomposition to fall into the pressure range of 0.1 atm⬍ pCO ⬍ 10 atm. Even by considering the uncertainties in the reaction rate constants and the limitation to a single kMC lattice, these results agree rather nicely with the reactor STM experiments by Hendriksen et al.,15 which were performed under similar temperature and pressure conditions 共T = 408 K, ptot = pCO + pO2 = 1.23 atm兲. Depending on the pressure ratio of oxygen and CO, Hendriksen et al. observed a change in the morphology of the surface, which was assigned to a change from an oxidic to a reduced surface structure and oxygen-rich feeds were required to stabilize the oxidic structure. The simulation results for the highest considered temperature of T = 600 K are shown in Fig. 5共c兲. We find that for this elevated temperature, the surface oxide is now actually stable up to rather sizable CO pressures. Only for CO pressures as high as pCO = 10 atm does the surface oxide start to decompose 共¯Ohol ⬍ 95% 兲, which already coincides almost with the border of its stability as determined in the constrained thermodynamics approach 共black vertical line兲. In the ‘‘phase’’ diagram in Fig. 4, it can be seen that for a temperature of T = 600 K and an oxygen pressure of pO2 = 1 atm, CO is not stabilized in large amounts as an adsorbate on the surface oxide. The CO is thus not readily available as an adsorbed reaction partner and the stability of the surface oxide is hardly affected by the ongoing catalytic CO2 formation. Up to the stoichiometric pressure ratio of pCO / pO2 = 2 : 1, no decomposition of the surface oxide structure occurs and, as apparent from Fig. 5共c兲, this result holds even in light of the estimated uncertainty of the underlying DFT energetics. Comparing the critical pCO / pO2 ratio determined for the decomposition onset in the temperature range T = 300– 600 K, we can thus clearly identify an increasing stability of the surface oxide with increasing temperature, which, at the highest temperatures studied, reaches well up to the catalytically most relevant feeds. Furthermore, we find that under these feeds, the simulated turnover frequencies for the intact surface oxide alone are already of a similar order of magnitude as those reported by Szanyi and Goodman42 for the Pd共100兲 surface under comparable gas-phase conditions. While a quantitative comparison is outside the scope of the present work, we note that contrary to the prevalent general preconception, at least this particular surface oxide is thus clearly not “inactive” with respect to the oxidation of CO. IV. SUMMARY We have employed first-principles kMC simulations to investigate the stability of the 冑5 surface oxide structure at Pd共100兲 against CO-induced decomposition under steadystate operation conditions of the CO oxidation reaction. The focus has been particularly set on the thin surface oxide, since this structure was identified as the most stable oxidic ‘‘phase’’ under catalytically relevant gas-phase conditions in a preceding constrained first-principles thermodynamics study.6 The developed kMC model describes the CO oxidation on the 冑5 surface oxide, accounting for all nonconcerted processes that are possible on the chosen kMC lattice. This includes 26 site- and element-specific adsorption, desorption, diffusion, and reaction processes. The respective kMC rate constants have been obtained from DFT total energy calculations together with harmonic transition state theory. Monitoring the onset of the surface oxide decomposition at increasing CO pressures, the central result of the kMC simulations is that, much in contrast to thicker bulklike oxide films, the stability of the 冑5 surface oxide can well extend to gas-phase conditions that are relevant for technological CO oxidation catalysis. While the accuracy of present-day DFT functionals does not permit us to conclude on precise values for the critical CO : O2 partial pressure ratio above which decomposition sets in, our results undoubtedly show that at ambient pressures this ratio is close to the most interesting stoichiometric feed conditions 共pCO : pO2 = 2 : 1兲 and will, furthermore, shift decisively toward more CO-rich conditions with increasing temperature. On the basis of these results, we conclude that the surface oxide structure can actually be present under catalytic reaction conditions at ambient pressures and our simulated turnover frequencies indicate that it is then also catalytically active toward the oxidation of CO. For the catalytically most relevant feeds, the system appears, furthermore, to be rather close to a transition between the 冑5 surface oxide structure and a reactant covered Pd共100兲 surface. Particularly in stoichiometric to slightly O-rich feeds, even local fluctuations in both the temperature and the reactant partial pressures might then lead to significant local or global changes in the structure and composition of the surface. Under steady-state operation conditions, oscillations between these two states are thus conceivable, so that in its active state the catalyst surface might exhibit parts that correspond to Pd共100兲 covered by the reactants, as well as by patches of surface oxide, and potentially it is precisely the ongoing formation and decomposition of the oxidic structure that is key to understanding the catalytic function of this surface under such technologically relevant pressures. For a full understanding of the catalytic CO oxidation at the Pd共100兲 surface in corresponding 155410-11 PHYSICAL REVIEW B 77, 155410 共2008兲 ROGAL, REUTER, AND SCHEFFLER environments, it thus appears not to be sufficient to concentrate on either the reduced Pd共100兲 surface or the oxidic structure, but both surface states as well as the morphological transition between the two will have to be included in an appropriate model. *Present address: Van’t Hoff Institute for Molecular Sciences, University of Amsterdam, Nieuwe Achtergracht 166, 1018 WV Amsterdam, The Netherlands. 1 C. H. F. Peden and D. W. Goodman, J. Phys. Chem. 90, 1360 共1986兲. 2 H. Over and M. Muhler, Prog. Surf. Sci. 72, 3 共2003兲. 3 K. Reuter, Oil Gas Sci. Technol. 61, 471 共2006兲; http://ogst.ifp.fr 4 K. Reuter and M. Scheffler, Appl. Phys. A: Mater. Sci. Process. 78, 793 共2004兲. 5 K. Reuter and M. Scheffler, Phys. Rev. Lett. 90, 046103 共2003兲; Phys. Rev. B 68, 045407 共2003兲. 6 J. Rogal, K. Reuter, and M. Scheffler, Phys. Rev. B 75, 205433 共2007兲. 7 T. W. Orent and S. D. Bader, Surf. Sci. 115, 323 共1982兲. 8 S.-L. Chang and P. A. Thiel, J. Chem. Phys. 88, 2071 共1988兲. 9 S.-L. Chang, P. A. Thiel, and J. W. Evans, Surf. Sci. 205, 117 共1988兲. 10 G. Zheng and E. I. Altman, Surf. Sci. 504, 253 共2002兲. 11 E. Lundgren, J. Gustafson, A. Mikkelsen, J. N. Andersen, A. Stierle, H. Dosch, M. Todorova, J. Rogal, K. Reuter, and M. Scheffler, Phys. Rev. Lett. 92, 046101 共2004兲. 12 M. Todorova, E. Lundgren, V. Blum, A. Mikkelsen, S. Gray, J. Gustafson, Borg, J. Rogal, K. Reuter, J. N. Andersen, and M. Scheffler, Surf. Sci. 541, 101 共2003兲. 13 P. Kostelník, N. Seriani, G. Kresse, A. Mikkelsen, E. Lundgren, V. Blum, T. Šikola, P. Varga, and M. Schmid, Surf. Sci. 601, 1574 共2007兲. 14 J. Rogal, K. Reuter, and M. Scheffler, Phys. Rev. Lett. 98, 046101 共2007兲. 15 B. L. M. Hendriksen, S. C. Bobaru, and J. W. M. Frenken, Surf. Sci. 552, 229 共2004兲. 16 A. B. Bortz, M. H. Kalos, and J. L. Lebowitz, J. Comput. Phys. 17, 10 共1975兲. 17 D. T. Gillespie, J. Comput. Phys. 22, 403 共1976兲. 18 A. F. Voter, Phys. Rev. B 34, 6819 共1986兲. 19 H. C. Kang and W. H. Weinberg, J. Chem. Phys. 90, 2824 共1989兲. 20 K. A. Fichthorn and W. H. Weinberg, J. Chem. Phys. 95, 1090 共1991兲. 21 P. Ruggerone, C. Ratsch, and M. Scheffler, in Growth and Properties of Ultrathin Epitaxial Layers, edited by D. A. King and D. P. Woodruff, The Chemical Physics of Solid Surfaces Vol. 8 ACKNOWLEDGMENTS The EU is acknowledged for financial support under Contract No. NMP3-CT-2003-505670 共NANO2兲, and the DFG for support within the priority program SPP1091. 共Elsevier Science, Amsterdam, 1997兲. S. Ovesson, A. Bogicevic, and B. I. Lundqvist, Phys. Rev. Lett. 83, 2608 共1999兲. 23 E. W. Hansen and M. Neurock, J. Catal. 196, 241 共2000兲. 24 E. W. Hansen and M. Neurock, Surf. Sci. 464, 91 共2000兲. 25 K. A. Fichthorn and M. Scheffler, Phys. Rev. Lett. 84, 5371 共2000兲. 26 P. Kratzer and M. Scheffler, Phys. Rev. Lett. 88, 036102 共2002兲. 27 K. Reuter, D. Frenkel, and M. Scheffler, Phys. Rev. Lett. 93, 116105 共2004兲. 28 K. Reuter and M. Scheffler, Phys. Rev. B 73, 045433 共2006兲. 29 A. Gross, Surf. Sci. Rep. 32, 293 共1998兲. 30 E. Sjöstedt, L. Nordström, and D. J. Singh, Solid State Commun. 114, 15 共2000兲. 31 G. K. H. Madsen, P. Blaha, K. Schwarz, E. Sjöstedt, and L. Nordström, Phys. Rev. B 64, 195134 共2001兲. 32 P. Blaha, K. Schwarz, G. K. Madsen, D. Kvasnicka, and J. Luitz, WIEN2K, Techn. Universität Wien, Austria, 2001. 33 J. P. Perdew, K. Burke, and M. Ernzerhof, Phys. Rev. Lett. 77, 3865 共1996兲. 34 J. Rogal and K. Reuter, in “Experiment, Modeling and Simulation of Gas-Surface Interactions for Reactive Flows in Hypersonic Flights,” p. 2-1–2-18, Educational Notes RTO-EN-AVT142, Neuilly-sur-Seine, 共2007兲. 35 C. Stampfl, H. J. Kreuzer, S. H. Payne, H. Pfnür, and M. Scheffler, Phys. Rev. Lett. 83, 2993 共1999兲. 36 K. Reuter, C. Stampfl, and M. Scheffler, in Handbook of Materials Modeling, edited by Sidney Yip 共Springer, Berlin, Heidelberg, 2005兲, Vol. 1, pp. 149–194. 37 D. De Fontaine, in Statistics and Dynamics of Alloy Phase Transformations, NATO Advanced Studies Institute Series 共Plenum, New York, 1994兲. 38 J. M. Sanchez, F. Ducastelle, and D. Gratias, Physica A 128, 334 共1984兲. 39 A. Zunger, in Statistics and Dynamics of Alloy Phase Transformations, NATO Advanced Studies Institute Series 共Plenum, New York, 1994兲. 40 A. Kiejna, G. Kresse, J. Rogal, A. De Sarkar, K. Reuter, and M. Scheffler, Phys. Rev. B 73, 035404 共2006兲. 41 R. M. Ziff, E. Gulari, and Y. Barshad, Phys. Rev. Lett. 56, 2553 共1986兲. 42 J. Szanyi and D. W. Goodman, J. Phys. Chem. 98, 2972 共1994兲. 22 155410-12